Functionalized Metal-Organic Framework Catalysts for Sustainable Biomass Valorization

Currently, pristine and functionalized metal-organic frameworks (MOFs) are introduced in heterogeneous catalysis for biomass upgrading owing to the specific texture properties including regular higher-order structure, high specific surface area, and the precisely tailored diversity.-e purpose of this review is to afford a comprehensive discussion of the most applications in biomass refinery. We highlight recently developed four types of MOFs like pristine MOFs and their composites, MOF-supported metal NPs, acid-functionalized MOFs, and biofunctionalized MOFs for production of green, sustainable, and industrially acceptable biomass-derived platform molecules: (1) upgrading of saccharides, (2) upgrading of furan derivatives, and (3) upgrading of other biobased compounds.


Introduction
Rapid population growth and enhanced living quality requirements led to an improvement in energy demand and fossil feedstocks containing coal, petroleum, and natural gas. Another mainstream of the current generation is the increasing motivation to protect the environment from greenhouse gas emissions aroused by the tremendous consumption of fossil fuels [1,2]. is concern is an irritation for the researchers for renewable and replaces sustainable resources instead of non-renewable fossil-based fuels. Because biomass is a green, highly abundant, and carbon-natural process available, it is served as a promising and replacing one to be transformed through bio-refinery and catalytic valorization into an extensive series of valueadded chemicals, which has a relatively low impact on the environment [3][4][5][6][7][8][9][10][11].
Various technologies including biological, thermal, and chemical procedures have been explored for biomass upgrading. Among those, chemical processes (e. g., dehydration, hydrolysis, esterification, alcoholysis, isomerization, and etherification) of biomass conversion have drawn increasing researchers' attention, which resulting in petrobased products. While reaction rates, high yields of target molecules depend on catalysts.
Metal-organic frameworks (MOFs), also identified as micro-and mesoporous coordination polymers (PCPs), are a class of crystalline porous materials produced by metal centers or metal-containing secondary building units (SBUs) and bi-or multimodal functional organic linkers [25,26]. MOFs are of particular research topics for biomass valorization owing to the proverbial texture properties such as changeable pore/cage size, high surface area, large cavity diameter and volume, the tunable diversity, and high hydrothermal stability [27]. In addition, the MOFs afford to functionalized anxious acid-base groups (-SO 3 H, -NH 2 , etc.), excellent support of active metal nanoparticles (Ru, Pt, Cu, etc. ) on particular sites, and immobilization of high-efficient homogeneous catalyst (POMs, ILs, et al.). e obtained functionalized MOFs could be an arbitrary choice application in diverse catalytic strategies with the existence of synergistic active moieties ( Figure 1).
Among more than 20,000 well-known MOFs, MIL (Material of Institut Lavoisier), consisting of rigid terephthalate organic linkers and trimeric octahedral metal-oxo clusters, possesses kinds of quasispherical mesoporous cages (20-35Å), with 5-20Å windows and large surface areas (2000-5900 m 2 /g). UiO (UiO for University of Oslo), zirconium terephthalate, which has 3D microporous cubic pore system and relatively high stability (∼500°C), is combined with large accessible pore volumes. ZIF (zeolitic imidazolate frameworks), having 3D structural feature with nanometre pore size and large Brunauer-Emmett-Teller (BET) surface area (<2000 m 2 /g), has been reported to act as a template/ precursor to give porous carbon.  [28]. e HMF and total reducing sugar molar yielding high up to 40.3% and 54.2% were achieved with 200°C, 4 h, respectively. e aluminum-based MOF acted as a reuse catalyst for three cycles without obvious activity loss, and the HMF yield (40.3%) decreased to 38.4%, which was ascribed to MIL-53(Al) mass weightlessness in cleaning proceeds and plugging of active sites by unexpected byproducts. e preparation of lactic acid and derivatives from carbohydrates are important processes in biomass valorization. Lactic acid is a worthy platform molecule for the development of degradable bioplastic manufacture and towards the preparation of multiple noticeable chemicals like acrylic acid, propylene glycol, 1,2-propanediol, poly(lactic acid) and linear esters (alkyl lactic acids). Two zeolitic imidazole frameworks (ZIFs) Zn-ZIF-8 and Co-ZIF-67 were synthesized and acted as a catalyst for the transformation of carbohydrates (sucrose, glucose, and fructose) to lactic acid derivatives for the first time [29]. e ZIFs processed by zeolite-type topology, 3D-porous rigid framework and high chemical and thermal stability are obtained facile, providing 42% methyl lactate using the prepared Zn-ZIF-8 for the eversmaller crystal particles and higher content of Lewis acidic. Reusability studies indicated the reduction of methyl lactate yields from 34.8% to 27.2% after the fourth recycling catalyzed by ZIF-8, on account of active site absence and structural difference. Furthermore, the metal node effect of catalysts M-MOF-74 (M = Co, Ni, Mg, and Zn) on the performance of the transformation of carbohydrates to methyl lactate was studied [30]. Among these, it expressed the optimal performance for 35% and 47% yields of the product based on glucose and sucrose under the optimal reaction conditions with 220°C and 6 h, respectively. Meanwhile, the Mg-MOF-74 catalyst exhibited excellent stability that could be reused three cycles without deactivation. Similarly, Huang et al. [31] revealed an efficient onepot conversion of fructose to lactic acid via catalyst Fe-MOF. Lactic acid yielding high up to 32% was achieved with fructose as the substrate, benefitting from the particular porous feature of catalyst MIL-100(Fe), while relatively low yields of 18% and 20% lactic acid were found with other MOFs, such as Cu-BTC and MIL-100(Cr), respectively. Derived from hexose-based carbohydrates including glucose, sucrose, inulin, and cellobiose, moderate lactic acid yields were effectively converted over MIL-100(Fe). e existed pores or active sites blockage and the absence of partial active sites and the catalytic performance of MIL-100(Fe) evidently reduced after the fourth recycle. Modifying the regeneration method of catalyst MIL-100(Fe), lactic acid yield maintained 28% from fructose.

MOFs for Biomass Valorization
In another work, the possible mechanism accounting for the preparation of methyl lactate with glucose as the reactant was revealed. MIL-101(Cr) combined with activated fly ash complex was developed to be effectual for furfural synthesis over xylose dehydration [32]. Compared to the bare MOF, 71% and 80% high yield and selectivity of furfural were acquired at optimized reaction conditions; the excellent performance was retained after ten times continuous recycling. e synergistic action of Cr Lewis acidic and -OH Brønsted acidic belonging to composite laid the foundations for application in other biomass valorization.

Upgrading of Furan Derivatives.
e catalytic oxidation of HMF providing a series of great value platform molecule for chemical engineering industries includes 2,5-diformylfuran (DFF), 5-hydroxymethylfuran-2-carboxylic acid, 2,5-dimethyltetrahydrofuran, and 5-ethoxymethylfurfural. e conversion and selectivity of the aforementioned molecules can be adjusted by regulating catalyst active sites' constitutions and experiment conditions. Lucarelli et al. [33] verified the oxidation process of HMF-DFF over Ni-based MOFs including Ni(BDP), Ni(BPEB), and Ni 3 (BTP) 2 , which were equipped with square planar and accessible metal centers. Among the base-free catalysts, Ni 3 (BTP) 2 exhibited the optimal catalytic activity, yielding 27% DFF under mild reaction conditions (120°C, 30 bar O 2 , in water). e satisfactory catalytic performance attributed to the accessibility of the metal centers, which depend on the crystal texture of the MOF. Following, an efficient MOF was applied in another conversion of one-pot two steps processes, which was investigated to prepare furilydenepropanenitrile derivatives, the key polymer basic entities [34]. e first oxidation procedure of HMF was explored by Febased MOFs (MIL-100(Fe), Cu-based MOF, Fe-HY zeolite, and Fe salts with 2,2,6,6-tetramethylpiperidine-1-oxide (TEMPO) acting as cocatalyst, NaNO 2 serving as an additive, and O 2 as the terminal oxidant. Post-treated by NH 4 F, MIL-100(Fe) explained the highest catalytic activity, giving a full yield of DFF converted from HMF, which ascribe to the existence of accessibility of Fe(III) active sites for reactants. e following Knoevenagel condensation step of DFF catalyzed by malononitrile or ethyl cyanoacetate was carried out under the basic medium.
rough aldol condensation, aldehydes and ketones react to provide high-value-added products from simple and inexpensive ones. On account of which, Kikhtyanin et al. [35] contrasted the catalytic effect of Lewis acidic MOFs (Cu-BTC, Fe-BTC) with zeolites including both Lewis acidity and Brønsted acidity to inquire the aldol condensation reaction of furfural with acetone. As demonstrated, acidic sites have the advantage to proceed aldol condensation rather than basic ones. It is worth noting that catalysts possessing weak Brønsted acidity, which are obtained by the mutual effect of Fe 3+ with coordinated H 2 O or the presence of structural defects, showed the best performance at 100°C. e oxidative condensation reaction of furfural with alcohols-O 2 can promote double-carbon molecules to synthesize longer hydrocarbon chains acting as transport biofuels. In recent years, furfural reacting with alcohol to proceeding the aerobic oxidative condensation was explored by multiple Co-MOF catalysts [36]. Generally, two tactics were surveyed for the production of effective catalytic sites in MOFs: (1) removal of a coordinated small organic molecule or water molecules at 300°C, issuing in exposed and available metal active species; (2) thermolysis at 700°C, obtaining carbon-matrix nanometer and porous composites. Both types of Co-MOF exhibited satisfactory catalytic activity in the oxidative condensation with 84.9% and 99% furfural conversion and selectivity under optimal reaction conditions.
Except that, Zr-based MOFs (UiO-66 or UiO-66-NH 2 ), were further examined on the esterification reaction of levulinic acid with the amount of biomass-derived various alcohols [37]. e gained catalytic performances are comparable to have published heterogeneous acidic catalysts' activities, and the data exhibit the excellent activity, thanks to the synthesis conditions, defect sites, and particle size in these MOFs.

Upgrading of Other Biobased Compounds.
Because of the consumption of petrochemical energy, the development of transformation of biomass to biodiesel over esterification and transesterification reaction become an attractive topic. Larasati et al. [38] examined the catalytic performance of the synthesized Zr 4+ -BTC based MOF by the solvothermal and reflux method for the esterification of palmitic acid and ethanol. e solvothermal prepared MOF affords the maximum 69.2% palmitic acid conversion with 0.6% catalyst loading. In addition, Zr-MOFs, like UiO-66 and UiO-66-NH 2 , are also inquired as heterogeneous acids for fatty acids with short-chain alcohols to carry out the esterification reaction [39]. With the optimized reaction condition, excellent outputs of fatty acid alkyl esters (94-99%) were provided over the superior UiO-66-NH 2 , which was ascribed to cooperative acid-base catalytic properties. e investigation further proved that Zr-MOFs possess the potential to catalyze other biobased feedstock conversions. To reduce the dependence on petroleum resources, c-valerolactone (GVL) as the sustainable production from renewable biomass was identified as significant target chemicals. 5 wt.% Ru/MIL-101(Cr) catalyst afforded above 99% GVL yield with 100% conversion of levulinic acid compared to a Ru/zeolite catalyst at mild reaction conditions (70°C, 5 h, 1.0 MPa H 2 pressure) [43]. e higher catalytic performance is due to the synergistic effect between the MIL-101(Cr) supporter and the well-dispersed Ru sites.

Upgrading of Other Biobased Compounds.
e oxidation of glycerol provides sustainable routes for value-added chemicals, such as polyglycerol, glyoxylic acid, and glyceraldehyde [44]. Li et al. [45] studied M-NPs/Fe-MIL-101 (M � Pd, Pd-Ce, Ce, and Au) for the production of dihydroxyacetone by adjusting the reaction time and metal types. Test results indicated that the longer reaction time better catalytic activity of the Pd-Ce NPs/Fe-MIL-101 for the glycerol oxidation to produce derivative dihydroxyacetone. Intriguingly, the modalism of Fe-MIL-101-NH 2 is slightly reliance on the preparation time, while the crystal structure maintained. With the MOF-supported metal-particles catalysts, bimetallic ones afforded higher yields of target compounds compared with the monometallic Pd-based MOF.
Furthermore, palladium nanocatalyst incorporated the hybrid support constituting the novel Pd/PRGO/Ce-MOF, among which the supports composed of Ce-MOF crystals and partially reduced graphene oxide (PRGO) nanosheets [46]. Results highlighted the developed 5 wt.% Pd/PRGO/ Ce-MOF exhibited excellent catalytic performance for the transformation of vanillin to synthesize 2-methoxy-4methylphenol by successive hydrogenation-deoxygenation reactions. e desired performance is due to the reason of Pd nanoparticles' uniform dispersion on support and the existence of acidic active sites.

Acid-Functionalized MOFs
2.3.1. Upgrading of Saccharides. Utilization of renewable and abundant reserve resources like biomass caters to the development of sustainable production of chemicals. Biomass-derived saccharides (e.g., cellulose, sucrose, glucose, and fructose) can be catalyzed into bio-platform molecules, for instance, HMF was catalyzed and applied in medicine, fuel additives, and various fine chemicals which were applied to polymers and solvents [47,48]. Generally, fructose bearing a five-membered ring can be easily transformed into HMF by dehydration reaction, while glucose with a more stable six-membered ring is the direct product of lignocellulosic biomass and is cost efficient; its conversion and application remain challenging. e transformation of glucose-HMF process carries out through two steps, I) the isomerization reaction of glucose over Lewis acid to fructose and II) the dehydration process for HMF catalyzed by Brønsted acid [49]. Considering the catalytic activity, the catalyst combined Brønsted and Lewis acidity would be superior over the separated ones.
In view of the situation, Oozeerally et al. [50] investigated the prominent stable and strong acidic UiO-66-MSBDC catalyst for the transformation of glucose-HMF, among which the catalyst was prepared via partially substituting the organic linker of UiO-66 by MSBDC. For the obtained catalyst constructed with Lewis (Zr 4+ ) and Brønsted (-SO 3 H) acidities, the synergistic effect of the catalyst guaranteed prominent catalytic performance for the production of HMF in aqueous solution under optimized reaction condition.
Considering a more stable pyranose form of glucose reduces the efficiency of HMF yield; Oozeerally et al. [49] and Yabushita et al. [50] demonstrated PO 4 /NU as an efficient catalyst for the production of HMF derived from glucose, which is synthesized by partial phosphate modification of Zr-MOF NU-1000 to provide strong acidic sites to accomplish the glucose-to-HMF conversion. Results verified the maximum yield of 64% HMF with 1 mM glucose concentration in water/ 2-propanol hybrid medium. e high yield and selectivity attributed to the reduced Lewis acidity combined Brønsted acidity, which are favorable for the glucose-fructose isomerization and the followed dehydration process.
Similarly, selective products of glucose catalyzed by nitro-or sulfo-modified functionalized MIL-101(Cr) catalysts and MOF derivatives were explored in depth [48]. Research has found that the MIL-101(Cr)-SO 3 H catalyst afforded the highest yield (29%) of HMF derived from glucose with 24 h, which is the maximum value over MOF so far. e solvent effect was studied and it was revealed that the distribution of the products over MIL-SO 3  Lewis and Brønsted acidity, which was evaluated for glucose conversion to synthesize HMF with optimized reaction conditions and GVL-combined 10 wt.% water acted as the reaction medium [52]. e HMF yield reaching up to 45% with full conversion of glucose was achieved with Cr 3+ centers as Lewis acid and -SO 3 H as the Brønsted one. e wonderful catalytic performance ascribed to the synergistic effect of Lewis and Brønsted acid and combined solvents, and the solvent effect was further proved by kinetic reactions, which revealed that the isomerization step obeyed second-order kinetics and GVL-H 2 O decreased the Ea value from 114 to 100.9 KJ mol − 1 .
With the same functionalized MOF-SO 3 H, Chen et al. prepared various sulfonic acid-functionalized MOFs using the postsynthetic modification method of functionalized organic linkers by chlorosulfonic acid, realizing the fructose dehydration for HMF production (Figure 2). [53]. e grafting level of -SO 3 H groups affected the Brønsted acid density and the acidic strength of catalysts and further determined the output of the ultimate product HMF. e HMF yield reached up to 90% with the full conversion of fructose with the optimized MIL-101(Cr)-SO 3 H (15.0%) catalyst, which is superior to the UiO-66 and MIL-53. About 55 KJ mol − 1 activation energy was achieved through kinetic reaction, and at the same time, the fructose-HMF conversion process possibly followed the pseudo-first-order kinetics. Results showed that the product yields did not remain stable after five recycles, which indicated that the catalyst channel may accumulate oligomeric products derived from side reaction.
Followed, Hu et al. [54] directly synthesized the high stability and strong Brønsted acidity NUS-6, including two types of Zr and Hf clusters with modulated hydrothermal (MHT) approach. e novel catalysts NUS-6(Zr) and NUS-6(Hf ) possessed high specific surface areas of 550 and 530 m 2 g − 1 , respectively, which increases the interaction sites between reactants and active acidic sites. As a consequence, the NUS-6(Hf) MOF exhibited the optimal HMF yield of 98% in the fructose dehydration process, which was also attributed to the strong Brønsted acidity and the appropriate pore size that suppressed secondary reactions.
Furthermore, the acidic adjustability played an increasing remarkable role in the catalytic conversion of biomass. A hybrid MOF-based solid acidic catalyst PVP-HNTs@UiO-66-SO 3 H-x prepared with polyvinylpyrrolidone-modified halloysite nanotubes incorporated in a -SO 3 H group-functionalized UiO-66(Zr) revealed good catalytic property for fructose dehydration reaction with high HMF yield (92.4%) [55]. e acidic site density in the PVP-HNTs@UiO-66-SO 3 H can be tuned by altering the dosage of support and -SO 3 H groups. e catalyst can be facilely and effectively reused for successive five cycles without obvious loss in its activity and stability.

Upgrading of Furan Derivatives.
Research has shown that c-valerolactone (GVL) can act as a plasticizer, fuel additive for gasoline, aviation kerosene that can reduce the dependence on the petrochemical energy, and can be further converted to liquid long-chain hydrocarbon fuels for diesel. Considering this situation, Kuwahara et al. [56] developed an SO 3 H-functionalized Zr-MOF (UiO-66-Sx) for the production of GVL through converted hydrogenation from levulinic acid and its corresponding esters. Owing to the strong connection of Brønsted acidic -SO 3 H groups and Lewis-basic Zr 6 O 4 (OH) 4 clusters existed in the UiO-66 framework, the highest yield of GVL reaches up to 85% at 140°C. Meanwhile, UiO-66-S 60 containing 60 mol% fraction of -SO 3 H maintained relatively high BET surface area although functionalization leads to the reduction of crystallinity and BET surface area.
In addition, among the various studies on biomass valorization, the preparations of alkyl levulinates have attracted much attention in recent years. e transformation of furfuryl alcohol to ethyl levulinate was investigated with the SO 3 H-functionalized Cr-MOF MIL-101(Cr)-SO 3 H in ethanol ( Figure 3). [57] e as-prepared catalyst materials possessed special textural properties including high BET surface area, porous mesopore size, high hydrothermal/ chemical stability, and increased approachability of -SO 3 H Brønsted acidic sites. By the reason of the aforementioned satisfying characteristics, the catalyst MIL-101(Cr)-SO 3 H afforded good catalytic performance with a yield of 79.2% ethyl levulinate and 100% furfuryl alcohol conversion. Reusability experiments further proved the material stability with a slight loss of activity was showed.

Upgrading of Other Biobased Compounds.
Esters, the products of esterification, are widely applied for fragrances, lubricants, plasticizers, drugs, pharmaceuticals, and solvents. At the same time, dehydration of alcohol is a significant reaction to industrial development. Based on these, novel acid-functionalized MOF attracted numerous interests for the application in various areas. Hasan et al. [58] published the esterification reaction of oleic acid with MeOH to produce biodiesel using porous and strong acidic MIL-101(Cr)-SO 3 H in order to improve process efficiency and energy conservation. Remarkably, the maximum yield of methyl oleate up to 93% was gained within only 20 min by microwave heating, which was superior compared to the conventional heating with 10 h, resulting in similar product yield.
For the sake of modification of vegetable oils in a friendly and environmentally pattern, the high catalytic activity and excellent stability Cs 2.5 H 0.5 PW 12 O 40 @ UiO-66 were synthesized by facile solvothermal approach, which method encapsulated the Keggin-type Cs 2.5 H 0.5 PW 12 O 40 heteropolyacid into microporous UiO-66 crystal with enhanced Lewis acidity [59]. Results demonstrated that functionalized MOF exhibited good catalytic activity for soybean oil proceeding the acidolysis reaction towards low-calorific lipids. e best catalytic activity attributed to the synergistic effect of acid sites and the well-dispersed Ru nanoparticles, which promoted hydrolysis and subsequent C-C bond fragmentation and hydrogenation reaction, respectively. Leaching of catalyst active species in the recycle reaction can be explained by partial decomposition of NENU-3, which further affects the decrease in product yields to a certain extent.  6 Advances in Polymer Technology A one-pot hydrogenation conversion procedure of methyl levulinate into GVL was investigated with a bifunctional hybrid catalyst preparing by metallic Ru nanoparticles incorporated on functionalized UiO-66-SO 3 H [62]. Under mild reaction conditions (0.5 MPa, 80°C, 4 h), 81% high yield of GVL was attained owing to the synergistic effect of Ru NPs and plenty of Brønsted acidic sites of catalysts that promoted the intermediates converted efficiently. Reusability experiments demonstrated the stability of the catalyst with five coherent times maintained no remarkable loss of activity, while the significantly decreased catalytic performance of two-stage processes further confirmed the indispensable role of -SO 3 H groups.

Bifunctionalized
A hybrid Pd/UiO-66@SGO (SGO-sulfonated graphene oxide) material was studied for the one-pot transformation of monosaccharides into 2,5-dimethylfuran [63], which was prepared by supporting the Pd nanoparticles on UiO-66@ SGO. e abundant Brønsted acidity existing in UiO-66@ SGO guaranteed the high yield of HMF, while the succeeding hydrogenation/hydrogenolysis for the product 2,5dimethylfuran was catalyzed by uniform dispersed Pd nanoparticles. Direct conversion from fructose afforded the maximum 2,5-dimethylfuran yield of 70.5 mol% under the optimized reaction conditions, while surprisingly, glucose acted as the substrate provided 45.3% mol yield for 2,5dimethylfuran. A bifunctional Pd/MIL-101(Al)-NH 2 was explored for the selective hydrogenation of HMF to produce 2,5-dihydroxymethyl-tetrahydrofuran (DHMTHF) [65]. e catalyst was prepared via direct anionic exchange procedure and then the reduction step was introduced for the Pd nanoparticles immobilized on MIL-101(Al)-NH 2 . e existence of isolated amine groups of the catalyst guaranteed the constitution of well dispersion of Pd nanoparticles avoiding the aggregation of Pd NPs. With the explored catalyst, the conversion process HMF-DHMF (2,5-dihydroxymethyl-furan)-DHMTHF afforded a 96% high yield of DHMTHF and 100% coversion of HMF at only (30°C). e excellent catalytic activity partially ascribed to the hydrophilic nature of DHMF and the interaction of DHMF and MOF, which further promoted the transformation of DHMF to the target product. e investigation exploited the perspectives of functionalized Al-MOF-NH 2 for sustainable biomass valorization.

Upgrading of Other Biobased Compounds.
As the ordinary component of lignin-derived bio-oil, vanillin was converted through hydrodeoxygenation reaction using bifunctional Pd/SO 3 H-MIL-101(Cr), which was developed by immobilization of Pd nanoparticles on mesoporous functionalized Cr-MOF [66]. e existing Brønsted acidic groups -SO 3 H of the MOF acted as the activator of the reactants guaranteeing the catalytic efficiency. Results showed that the 2 wt.% Pd/MIL-101(Cr)-SO 3 H catalyst indicated excellent capability in the hydrodeoxygenation of vanillin for the product 2-methoxy-4-methylphenol. Meanwhile, the reusability of the catalyst proved the stability that can be continuously reused for no less than seven recycles without a decrease of catalytic effect. Comparable studies of the hydrodeoxygenation of vanillin were published with a similar catalyst Pd@NH 2 -UiO-66, which was prepared by ultramicro Pd nanoparticles (1.5-2.5 nm) incorporated in a basic-functionalized MOF (NH 2 -UiO-66) [67]. Until now, the maximum 100% yield of 2-methoxy-4-methylphenol was obtained higher than 2 wt.% Pd@NH 2 -UiO-66 with mild reaction conditions as 0.5 MPa and 100°C for 60 min. e synergistic effect of uniform Pd sites and the NH 2 -UiO-66 support played a critical role in the wonderful catalytic performance of Pd@NH 2 -UiO-66. e comparison study of Pd/UiO-66 and NH 2 -functionalised Pd/UiO-66 catalysts was conducted for phenol hydrogenation to prepare cyclohexanol [68]. Interestingly, the introduction of NH 2 groups verified a destroyed crystalline structure in UiO-66, providing weak chemical interaction between Zr and Pd in prepared Pd-UiO-66-NH 2 . Based on that, the Pd-UiO-66 catalyst exhibited preferable catalytic performances in phenol hydrogenation than Pd-UiO-66-NH 2 with complete conversion of phenol for only 2 h in 120°C. Chemical kinetic results exhibited that the activation energies with Pd-UiO-66 and Pd-UiO-66-NH 2 are 50.44 ± 3.20 and 43.11 ± 5.98 kJ/mol, respectively, which further proved the aforementioned conclusion. Advances in Polymer Technology e presence of oxygen-containing C16-C18 fatty acids causes polymerization, weak oxidation stability, and low calorific value, even when cannot efficiently utilize the algaederived bio-oil for transportation fuel. Considering this, Fang et al. [69] researched the facile conversion of palmitic acid to hexadecane catalyzed by the bifunctional PTA@ PdCu@Fe III -MOF-5, which was prepared by immobilizing phosphotungstic acid into the MOF structure. e explored catalyst demonstrates an enhanced acidity and efficiently facilitates palmitic acid for hexadecane with relatively high selectivity. e preferable catalytic activity was explained by its particular yolk-shell structural feature, increased acidity, and the superior supercritical fluid medium.

Determinant of MOF Catalytic Performance in Biomass
Valorization.
e multiplicity of metal centers and functional/nonfunctional organic ligands combined the chemical interactions grants MOFs to act as active catalysts, catalyst carriers, or catalyst precursors. Because of the stable SUB coordinated networks, MOFs possess adjustable pore size, high specific surface areas, and multiple topology structures compared to traditional heterogeneous solid catalysts.
Considering the conversion of biomass feedstocks which usually involves larger molecules, appropriate pore size, and morphologies which are needed to be serious-minded adjusted for the reactants, intermediates and productions efficiently diffuse towards catalytic active sites. For example, Li et al. [45] demonstrated that the morphology of Fe-MIL-101-NH 2 can be ameliorated by altering the preparation time, resulting in desired catalytic activities in glycerol oxidation. e independent metal ions or clusters and functional/ nonfunctional organic ligands can afford required acid-base properties.
e unsaturated or defected metal centers in MOFs generally provide Lewis acidity. By the reason of Lewis acidic, MOFs can act as heterogeneous acid catalysts for glucose isomerization into fructose [50]. Owing to the necessity of Brønsted acid in various biomass-upgrading reactions, several feasible approaches have been explored to introduce Brønsted acidic functional sites onto specific sites of the MOFs [45,70]. Up to now, the functionalization of MOFs with Brønsted acid mainly including the post-synthetic modified method, [53] one-pot synthesis through organic ligands containing substituent groups [57] and active component supported on MOFs [60]. e functionalized MOFs integrate the superiorities of MOFs and encapsulated functional active sites facilitating cascade catalytic conversion for efficient biomass valorization (Scheme 1). e rigid coordination textural properties of frameworks are fatal determinants used as catalyst supports to synthesize highly stable heterogeneous catalysts. e easily regulated porous textures of MOFs supply strategies for the incorporation of catalytic metal NPs, avoiding agglomeration and enhancing catalytic performance [40,71].
Furthermore, MOFs have also been employed as matrixes for the production of carbon matrixes over pyrolysis procedure for supporting metal catalysts [72][73][74][75]. e obtained carbon templates can further work as a high S BET and stability carrier, which bore the generated metal nanoparticles, forming novel and well-dispersed active site catalysts. Wang et al. [73], tailoring the MOF-templated strategy, published an efficient bimetallic CuCo/C catalyst for the furfural conversion with the maximum 96.4% yield of furfuryl alcohol.

Conclusions and Perspectives
Taking the global warming impact into consideration, the sustainable and renewable resources such as biomass have become the hot research topic in the 21st century. With appropriate approaches (biological, thermal, or chemical processes), biomass can be derived into various value-added chemicals and fuels.
Addressing challenges in MOF preparation and application include concerns of availability, cost, toxicity, safety, and environmental impact, which are critical to evaluate the introduction of MOF materials for biomass upgrading. e exploitation of multifunctional solid catalysts with an abundance of acidic, basic, or redox-active sites is significant for performing superior reaction efficiency, notably in tandem biomass procedures. Several promising approaches investigated for the fixation of acid-base and redox  8 Advances in Polymer Technology functional groups on specific sites of the abovementioned materials were argued at great length. Eventually, the succeeding impacts of functionalization on one-pot tandem procedures and other procedures that generally generated in biorefineries were thoroughly argued. More interesting research endeavors are therefore needed to develop novel functionalized solid catalysts, with multiple active sites and particular morphologies. Although enormous procedures have been accomplished upon the investigation of effective functionalized heterogeneous catalysts for biomass upgrading, further enhancements are still essential on account of continuable and renewable manufacturing. ere are challenges needed to be faced towards MOF-based catalyst handy applied in biomass valorization. For instance, (i) the fertile preparation method for cost-efficient MOFs as one-pot synthesis precesses; (ii) more stable MOFs and active sites; and (iii) effective analysis of structure-function relationships. Hence, in the future investigation, we would focus on minimizing catalyst production costs, improving production yields and hydrothermal stability, tailoring the selectivity towards a target product, and enhancing efficient reusability.

Conflicts of Interest
e authors declare that there are no conflicts of interest regarding the publication of this paper.